The material structure also results in low shrinkage during cooling, and resistance to plastic deformation. The absence of grain boundaries, the weak spots of crystalline materials, leads to better resistance to wear and corrosion. Amorphous metals, while technically glasses, are also much tougher and less brittle than oxide glasses and ceramics. Amorphous metals can be grouped in two categories, as either non-ferromagnetic, if they are composed of Ln, Mg, Zr, Ti, Pd, Ca, Cu, Pt and Au, or ferromagnetic alloys, if they are composed of Fe, Co, and Ni. Thermal conductivity of amorphous materials is lower than that of crystalline metal. As formation of amorphous structure relies on fast cooling, this limits the maximum achievable thickness of amorphous structures. To achieve formation of amorphous structure even during slower cooling, the alloy has to be made of three or more components, leading to complex crystal units with higher potential energy and lower chance of formation. The atomic radius of the components has to be significantly different (over 12%), to achieve high packing density and low free volume. The combination of components should have negative heat of mixing, inhibiting crystal nucleation and prolonging the time the molten metal stays in supercooled state. The alloys of boron, silicon, phosphorus, and other glass formers with magnetic metals (iron, cobalt, nickel) have high magnetic susceptibility, with low coercivity and high electrical resistance. Usually the electrical conductivity of a metallic glass is of the same low order of magnitude as of a molten metal just above the melting point. The high resistance leads to low losses by eddy currents when subjected to alternating magnetic fields, a property useful for e.g. transformer magnetic cores. Their low coercivity also contributes to low loss. The superconductivity of amorphous metal thin films was discovered experimentally in the early 1950's by Buckel and Hilsch. For certain metallic elements the superconducting critical temperature "T"c can be higher in the amorphous state (e.g. upon alloying) than in the crystalline state, and in several cases "T"c increases upon increasing the structural disorder. This behavior can be understood and rationalized by considering the effect of structural disorder on the electron-phonon coupling. Amorphous metals have higher tensile yield strengths and higher elastic strain limits than polycrystalline metal alloys, but their ductilities and fatigue strengths are lower.